Dimensionality‒Band Gap‒Third-Harmonic Generation Property Relationship in Novel Main-Group Metal Iodates
Park, Geonju; Byun, Hye Ryung; Jang, Joon I.; Ok, Kang Min; Chemistry of Materials 32 (2020) 3621–3630; doi:10.1021/acs.chemmater.0c01054

data_4003532
_publ_section_title
;
 Dimensionality--Band Gap--Third-Harmonic Generation Property Relationship
 in Novel Main-Group Metal Iodates
;
_journal_issue                   8
_journal_name_full               'Chemistry of Materials'
_journal_page_first              3621
_journal_page_last               3630
_journal_paper_doi               10.1021/acs.chemmater.0c01054
_journal_volume                  32
_journal_year                    2020
_chemical_formula_moiety         'Ag3 I6 In O18'
_chemical_formula_sum            'Ag3 I6 In O18'
_chemical_formula_weight         1487.83
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                75.09(3)
_cell_angle_beta                 89.91(3)
_cell_angle_gamma                76.20(3)
_cell_formula_units_Z            2
_cell_length_a                   8.1160(16)
_cell_length_b                   10.426(2)
_cell_length_c                   11.110(2)
_cell_measurement_reflns_used    27441
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      33.548
_cell_measurement_theta_min      0.361
_cell_measurement_wavelength     0.71073
_cell_volume                     880.4(3)
_computing_cell_refinement       'HKL3000sm (Otwinowski & Minor, 1997)'
_computing_data_collection       'PAL BL2D-SMDC Program (Shin et. al, 2016)'
_computing_data_reduction        'HKL3000sm (Otwinowski & Minor, 1997)'
_computing_molecular_graphics    'Ortep for Windows (Farrugia, 2012)'
_computing_publication_material  'WinGX publication routines (Farrugia, 2012)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXS-2013/2 (Sheldrick, 2013)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.964
_diffrn_measured_fraction_theta_max 0.779
_diffrn_measurement_device_type  'Rayonix MX225HS CCD area detector'
_diffrn_measurement_method       'omega scan'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.63
_diffrn_reflns_av_R_equivalents  0.024
_diffrn_reflns_av_unetI/netI     0.03
_diffrn_reflns_Laue_measured_fraction_full 0.964
_diffrn_reflns_Laue_measured_fraction_max 0.779
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            15293
_diffrn_reflns_point_group_measured_fraction_full 0.964
_diffrn_reflns_point_group_measured_fraction_max 0.779
_diffrn_reflns_theta_full        22.21
_diffrn_reflns_theta_max         33.505
_diffrn_reflns_theta_min         1.685
_diffrn_source                   'PLSII 2D bending magnet'
_exptl_absorpt_coefficient_mu    10.822
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.822
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'HKL3000sm Scalepack(Otwinowski et.al,2003)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    5.612
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1304
_exptl_crystal_size_max          0.073
_exptl_crystal_size_mid          0.039
_exptl_crystal_size_min          0.012
_refine_diff_density_max         5.364
_refine_diff_density_min         -4.499
_refine_diff_density_rms         0.523
_refine_ls_extinction_coef       0.0032(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     260
_refine_ls_number_reflns         7726
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.064
_refine_ls_R_factor_all          0.0465
_refine_ls_R_factor_gt           0.0457
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0866P)^2^+7.0321P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1303
_refine_ls_wR_factor_ref         0.1312
_reflns_Friedel_coverage         0
_reflns_number_gt                7470
_reflns_number_total             7726
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            cm0c01054_si_002.cif
_cod_data_source_block           Ag3In(IO3)6
_cod_depositor_comments
;Adding full bibliography for 4003530--4003534.cif.

 Adding full bibliography for 4003530--4003534.cif.
;
_cod_database_code               4003532
_shelx_estimated_absorpt_t_min   0.506
_shelx_estimated_absorpt_t_max   0.881
_shelx_shelxl_version_number     2018/3